1. Preparation before welding
First cut off the worn bucket teeth from the digger gp bucket body, and then use an angle grinder to polish the place where the bucket teeth are installed. There should be no dirt, rust, and check carefully for cracks and other defects; use carbon arc on the bucket teeth to be welded Gouging out the groove and clean it with an angle grinder.
①First, use GBE309-15 electrode for surfacing welding on the bucket body (joint with bucket teeth). The electrode must be dried at 350℃ for 15h before welding. The welding current should be too large and the welding speed should be slightly slower to ensure the fusion zone. The nickel content is 5% to 6% to prevent the generation of martensite sensitive to cracks.
② Perform tack welding. After the bucket teeth are assembled in place, use a D266 electrode with a diameter of 32MM to perform two-sided symmetrical tack welding, and the length of the weld should not exceed 30MM. Water cooling and hammering immediately after welding.
③ Bottom welding. Use D266 electrode with a diameter of 32MM for bottom welding. Use small current, DC reverse polarity, intermittent welding, short section welding. Water cooling should be done in time every time welding is stopped, and the temperature of the interlayer should be controlled below 50℃.
④ Perform filler welding. After the bottom welding is completed, use D266 electrode with a diameter of 4MM for intermittent welding. The welding current is 160A. One electrode is divided into 3 to 4 times to complete the welding. When the welding is stopped, the welding bead must be cooled to 50℃ with water in time. Below, hammering is performed to eliminate stress and prevent carbide precipitation; each two layers are welded, the left and right welds are alternately welded to ensure the symmetry of the welding, until the weld foot reaches 16MM. Use a magnifying glass to check the cracks after each weld. If there are cracks, use carbon arc gouging to eliminate them before welding.
After the digger gp bucket body and bucket teeth were welded and repaired, after more than a year of use, the welds were still good. This method has high efficiency, low cost and good effect in repairing bucket teeth, and has certain practical value.
Contact Person: Mr. Tang
Alloy Steel Excavator Brush Rake , Excavator Landscape Rake High Strength
Wear Resistant Steel Excavator Brush Rake Standard With ISO 9001 Certification
High Reliability Excavator Brush Rake , Excavator Rake Attachment For Land Clearing
High Durability Excavator Land Clearing Rakes Easily Interchanges With Bucket
Non Rotatable Excavator Mechanical Grapple Tough Material High Working Strength
Red Color Excavator Rock Grapple Easy Operation Excellent Performance
Excavator Attached Mechanical Grapple , Q345B Excavator Timber Stone Grapple
Hydraulic Excavator Mechanical Grab Multifunctional Custom Service Available
Compact Excavator Mounted Vibro Hammer , Hydraulic Piling Hammers For Excavators
High Strength Hydraulic Pile Hammer For Driving And Extracting Various Shapes Piles
OEM Available Hydraulic Pile Hammer Excavator Attachment Long Service lifetime
Good Stability Hydraulic Pile Hammer Blue Color With ISO 9001 Certification